# Diffusionless transformations

﻿
Diffusionless transformations

Diffusionless transformations are a class of phase changes that do not occur by the long-range diffusion of atoms but rather by some form of cooperative, homogeneous movement of many atoms that results in a change in crystal structure. These movements are small, usually less than the interatomic distances, and the atoms maintain their relative relationships. The ordered movement of large numbers of atoms lead some to refer to these as "military" transformations in contrast to "civilian" diffusion-based phase changes. [D.A. Porter and K.E. Easterling, Phase transformations in metals and alloys, "Chapman & Hall", 1992, p.172]

The most commonly encountered transformation of this type is the martensitic transformation which, while being the best known, is actually only one subset of non-diffusional transformations. The marentitic transformation in steel represents the most economically important example of this category of phase transformations but an increasing number of alternatives, such as shape memory alloys, are leaving the bounds of pure scientific interest and having significant impact on day-to-day life.Fact|date=June 2008

Classification and definitions

When a structural change occurs by the coordinated movement of atoms (or groups of atoms) relative to their neighbors then the change is termed "displacive". This covers a broad range of transformations and so further classifications have been developed [Cohen 1979] .

The first distinction can be drawn between transformations dominated by "lattice-distortive strains" and those where "shuffles" are of greater importance.

Homogeneous lattice-distortive strains, also known as Bain strains, are strains that transform one Bravais lattice into a different one. This can be represented by a strain matrix S which transforms one vector, y, into a new vector, x:

:$y=Sx$

This is homogeneous as straight lines are transformed to new straight lines. Examples of such transformations include a cubic lattice increasing in size on all three axes (dilation) or shearing into a monoclinic structure.

Shuffles, as the name suggests, involve the small movement of atoms within the unit cell. As a result pure shuffles do not normally result in a shape change of the unit cell - only its symmetry and structure.

Phase transformations normally result in the creation of an interface between the transformed and parent material. The energy required to generate this new interface will depend on its nature - essentially how well the two structures fit together. An additional energy term occurs if the transformation includes a shape change since, if new phase is constrained by surrounding material, this may give rise to elastic or plastic deformation and hence a strain energy term. The ratio of these interfacial and strain energy terms has a notable effect on the kinetics of the transformation and the morphology of the new phase. Thus, shuffle transformations, where distortions are small, are dominated by interfacial energies and can be usefully separated from lattice-distortive transformations where the strain energy tends to have a greater effect.

A subclassification of lattice-distortive dispalcements can be made by considering the dilational and shear components of the distortion. In transformations dominated by the shear component it is possible to find a line in the new phase that is undistorted from the parent phase while all lines are distorted when the dilation is predominant. Shear dominated transformations can be further classified according to the magnitude of the strain energies involved compared to the innate vibrations of the atoms in the lattice and hence whether the strain energies have a notable influence on the kinetics of the transformation and the morpholgy of the resulting phase. If the strain energy is a significant factor then the transformations are dubbed "martensitic" and if it is not the transformation is referred to as "quasi-martensitic".

Martensitic transformation

The difference between austenite and martensite is, in some ways, quite small: while the unit cell of austenite is, on average, a perfect little cube, the transformation to martensite sees this cube distorted by interstitial carbon atoms that do not have time to diffuse out during displacive transformation, so that it is a tiny bit longer than before in one dimension and a little bit shorter in the other two. The mathematical description of the two structures is quite different, for reasons of symmetry (see external links), but the chemical bonding remains very similar. Unlike cementite, which has bonding reminiscent of ceramic materials, the hardness of martensite is difficult to explain in chemical terms.

The explanation hinges on the crystal's subtle change in dimension. Even a microscopic crystallite is millions of unit cells long. Since all of these units face the same direction, distortions of even a fraction of a percent become magnified into a major mismatch between neighboring materials. The mismatch is sorted out by the creation of a myriad of crystal defects, in a process reminiscent of work hardening. As in work-hardened steel, these defects prevent atoms from sliding past one another in an organized fashion, causing the material to become harder.

Shape memory alloy also has surprising mechanical properties, that were eventually explained by an analogy to martensite. Unlike the iron-carbon system, alloys in the nickel-titanium system can be chosen that make the "martensitic" phase thermodynamically stable.

Pseudomartensitic transformation

In addition to displacive transformation and diffusive transformation, a new phase transformation that involves displasive sublattice transition and atomic diffusion was discovered using a high-pressure x-ray diffraction system. [Jiuhua Chen, Donald J. Weidner, John B. Parise, Michael T. Vaughan, and Paul Raterron, (2001) [http://prola.aps.org/abstract/PRL/v86/i18/p4072_1 Observation of Cation Reordering during the Olivine-Spinel Transition in Fayalite by In Situ Synchrotron X-Ray Diffraction at High Pressure and Temperature] "Phys. Rev. Lett", 86, pp. 4072–4075.] The new transformation mechanism has been christened a pseudomartensitic transformation. [Kristin Leutwyler [http://www.sciam.com/article.cfm?articleID=000E8826-A6AF-1C5E-B882809EC588ED9F New phase transition] "Scientific American", May 2, 2001.]

References

* [http://www.msm.cam.ac.uk/phase-trans/2002/martensite.html Extensive resources from Cambridge University Press]
* [http://www.aem.umn.edu/people/faculty/shield/hane/tet.html The cubic-to-tetragonal transition]

Wikimedia Foundation. 2010.

### Look at other dictionaries:

• Diffusionless transformation — Diffusionless transformations classifications A diffusionless transformation is a phase change that occurs without the long range diffusion of atoms but rather by some form of cooperative, homogeneous movement of many atoms that results in a… …   Wikipedia

• Phase transition — This diagram shows the nomenclature for the different phase transitions. A phase transition is the transformation of a thermodynamic system from one phase or state of matter to another. A phase of a thermodynamic system and the states of matter… …   Wikipedia

• Martensite — For the transformation, see Diffusionless transformations. Iron alloy phases Ferrite (α iron, δ iron) A …   Wikipedia

• Grain boundary — A grain boundary is the interface between two grains in a polycrystalline material. Grain boundaries disrupt the motion of dislocations through a material, so reducing crystallite size is a common way to improve strength, as described by the Hall …   Wikipedia

• Martensit — ist ein hartes, ferromagnetisches und metastabiles Gefüge in Metallen, das diffusionslos und athermisch durch eine kooperative Scherbewegung aus dem Ausgangsgefüge entsteht. Dabei muss das Material von der Temperatur einer Hochtemperaturphase… …   Deutsch Wikipedia

• Shape-memory alloy — A shape memory alloy (SMA, smart metal, memory metal, memory alloy, muscle wire, smart alloy) is an alloy that remembers its original, cold forged shape: returning the pre deformed shape by heating. This material is a lightweight, solid state… …   Wikipedia

• Shape memory alloy — A shape memory alloy (SMA, also known as a smart alloy, memory metal, or muscle wire) is an alloy that remembers its shape, and can be returned to that shape after being deformed, by applying heat to the alloy. When the shape memory effect is… …   Wikipedia